# Electronic Supplementary Material (ESI) for Journal of Materials Chemistry C.
# This journal is © The Royal Society of Chemistry 2023

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_I
_database_code_depnum_ccdc_archive 'CCDC 2259432'
loop_
_audit_author_name
_audit_author_address
'Angel Arevalo Lopez'
;CNRS UCCS, University of Lille
France
;
_audit_update_record             
;
2023-04-27 deposited with the CCDC.	2023-06-15 downloaded from the CCDC.
;
_publcif_datablock.id            {74acaf3a-2904-42f3-a9dd-46513829ff24}

#=======================================================================

# 5. CHEMICAL DATA

_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_formula_moiety         ?
_chemical_formula_structural     ?
_chemical_formula_analytical     ?
_chemical_formula_iupac          ?
_chemical_formula_sum            'Mn V O3'
_chemical_formula_weight         153.9
_chemical_melting_point          ?
_chemical_compound_source        ?
_chemical_absolute_configuration .

#=======================================================================

# 6. CRYSTAL DATA

_symmetry_cell_setting           triclinic
_symmetry_space_group_name_H-M   'P -1'
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_Int_Tables_number      2

loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -x,-y,-z

_cell_length_a                   5.0177(7)
_cell_length_b                   5.0513(7)
_cell_length_c                   5.5210(8)
_cell_angle_alpha                116.679(6)
_cell_angle_beta                 90.044(6)
_cell_angle_gamma                118.924(5)
_cell_volume                     105.10(3)



_cell_formula_units_Z            2

_cell_measurement_temperature    293
_cell_special_details            ?

_exptl_crystal_density_diffrn    4.8621

_exptl_crystal_F_000             144

_exptl_absorpt_coefficient_mu    5.185

_cell_measurement_reflns_used    5076
_cell_measurement_theta_min      3.39
_cell_measurement_theta_max      23.66
_exptl_crystal_description       block

#=======================================================================

# 7. EXPERIMENTAL DATA



_diffrn_ambient_temperature      293

_diffrn_radiation_type           'Ag K\a'
_diffrn_radiation_source         'X-ray tube'
_diffrn_radiation_wavelength     0.56086

_diffrn_measurement_device_type  'X8 Bruker'
_diffrn_reflns_number            5076
_diffrn_reflns_theta_min         3.39
_diffrn_reflns_theta_max         23.66
_diffrn_reflns_theta_full        21.74
_diffrn_measured_fraction_theta_max 0.94
_diffrn_measured_fraction_theta_full 0.96
_diffrn_reflns_av_R_equivalents  0.037
_diffrn_reflns_av_unetI/netI     0.0234
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_k_max       6
_diffrn_reflns_limit_l_min       -7
_diffrn_reflns_limit_l_max       7
_diffrn_reflns_reduction_process ?



_diffrn_radiation_probe          x-ray

#=======================================================================

# 8. REFINEMENT DATA

_refine_special_details          ?

_reflns_number_total             604
_reflns_number_gt                544
_reflns_threshold_expression     I>3σ(I)

_refine_ls_structure_factor_coef F
_refine_ls_R_factor_gt           0.0318
_refine_ls_wR_factor_gt          0.0452
_refine_ls_R_factor_all          0.0318
_refine_ls_wR_factor_ref         0.0452
_refine_ls_goodness_of_fit_ref   2.63
_refine_ls_goodness_of_fit_gt    2.63
_refine_ls_restrained_S_gt       ?
_refine_ls_restrained_S_all      ?
_refine_ls_number_reflns         544
_refine_ls_number_parameters     47
_refine_ls_number_restraints     0
_refine_ls_number_constraints    0
_refine_ls_weighting_scheme      sigma
_refine_ls_weighting_details     w=1/(σ²(F)+0.0001F²)

_refine_ls_shift/su_max          0.0206
_refine_ls_shift/su_mean         0.0071
_refine_diff_density_max         1.75
_refine_diff_density_min         -0.72
_refine_ls_extinction_method     
'B-C type 1 Gaussian isotropic (Becker & Coppens, 1974)'
_refine_ls_extinction_coef       320(80)


loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Mn 0.2704 0.4681 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
O 0.0056 0.0036 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
V 0.2276 0.3376 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'







#=======================================================================

# 9. ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_adp_type
_atom_site_U_iso_or_equiv
_atom_site_site_symmetry_multiplicity
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Mn1 Mn 0.64890(12) 0.28595(15) 0.42166(13) Uani 0.0090(4) 2 1 d . . .
V1 V -0.14533(13) -0.28822(17) 0.04681(15) Uani 0.0062(4) 2 1 d . . .
O1 O 0.5762(6) -0.2169(7) 0.2255(6) Uani 0.0092(15) 2 1 d . . .
O2 O 0.2210(5) 0.1673(7) 0.2342(6) Uani 0.0092(15) 2 1 d . . .
O3 O 0.9684(6) 0.5195(7) 0.2315(6) Uani 0.0076(14) 2 1 d . . .








#=======================================================================

# 10. MOLECULAR GEOMETRY


loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Mn1 Mn1 . 2_656 3.0654(14) ?
Mn1 Mn1 . 2_666 3.0175(13) ?
Mn1 Mn1 . 2_766 2.9638(15) ?
Mn1 V1 . 1_666 2.9639(16) ?
Mn1 O1 . . 2.095(4) ?
Mn1 O1 . 2_656 2.329(3) ?
Mn1 O2 . . 2.058(3) ?
Mn1 O2 . 1_655 3.283(3) ?
Mn1 O2 . 2_666 2.281(3) ?
Mn1 O3 . . 2.085(3) ?
Mn1 O3 . 2_766 2.191(3) ?
V1 V1 . 2_445 3.0250(15) ?
V1 V1 . 2_545 2.9997(14) ?
V1 V1 . 2_555 2.8491(15) ?
V1 O1 . 1_455 1.796(3) ?
V1 O1 . 2_545 2.139(2) ?
V1 O2 . . 1.874(2) ?
V1 O2 . 2_555 2.000(4) ?
V1 O3 . 1_445 1.932(4) ?
V1 O3 . 2_655 1.977(3) ?
O1 O1 . 2_645 2.540(4) ?
O1 O1 . 2_656 3.199(4) ?
O1 O2 . 1_545 2.761(5) ?
O1 O2 . . 3.195(6) ?
O1 O2 . 1_655 2.842(4) ?
O1 O2 . 2_655 2.805(5) ?
O1 O2 . 2_656 3.012(5) ?
O1 O3 . 1_445 2.681(4) ?
O1 O3 . 1_545 2.867(6) ?
O1 O3 . . 3.243(5) ?
O1 O3 . 2_655 2.942(4) ?
O1 O3 . 2_766 3.056(3) ?
O2 O2 . 2_555 2.627(4) ?
O2 O2 . 2_666 3.127(3) ?
O2 O3 . 1_445 2.874(5) ?
O2 O3 . 1_455 2.641(6) ?
O2 O3 . . 3.286(4) ?
O2 O3 . 2_655 2.889(4) ?
O2 O3 . 2_666 3.061(4) ?
O3 O3 . 2_765 2.507(5) ?
O3 O3 . 2_766 3.084(5) ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
Mn1 Mn1 Mn1 2_656 . 2_666 112.28(3) ?
Mn1 Mn1 Mn1 2_656 . 2_766 116.10(4) ?
Mn1 Mn1 V1 2_656 . 1_666 78.12(3) ?
Mn1 Mn1 O1 2_656 . . 49.38(9) ?
Mn1 Mn1 O1 2_656 . 2_656 43.07(9) ?
Mn1 Mn1 O2 2_656 . . 94.53(10) ?
Mn1 Mn1 O2 2_656 . 1_655 95.64(7) ?
Mn1 Mn1 O2 2_656 . 2_666 115.48(10) ?
Mn1 Mn1 O3 2_656 . . 148.34(11) ?
Mn1 Mn1 O3 2_656 . 2_766 77.58(9) ?
Mn1 Mn1 Mn1 2_666 . 2_766 114.04(3) ?
Mn1 Mn1 V1 2_666 . 1_666 74.53(3) ?
Mn1 Mn1 O1 2_666 . . 146.98(8) ?
Mn1 Mn1 O1 2_666 . 2_656 75.20(10) ?
Mn1 Mn1 O2 2_666 . . 49.07(8) ?
Mn1 Mn1 O2 2_666 . 1_655 151.19(7) ?
Mn1 Mn1 O2 2_666 . 2_666 42.97(8) ?
Mn1 Mn1 O3 2_666 . . 99.30(11) ?
Mn1 Mn1 O3 2_666 . 2_766 113.41(9) ?
Mn1 Mn1 V1 2_766 . 1_666 74.60(2) ?
Mn1 Mn1 O1 2_766 . . 98.93(8) ?
Mn1 Mn1 O1 2_766 . 2_656 116.07(7) ?
Mn1 Mn1 O2 2_766 . . 149.36(11) ?
Mn1 Mn1 O2 2_766 . 1_655 42.45(4) ?
Mn1 Mn1 O2 2_766 . 2_666 76.27(7) ?
Mn1 Mn1 O3 2_766 . . 47.61(9) ?
Mn1 Mn1 O3 2_766 . 2_766 44.67(8) ?
V1 Mn1 O1 1_666 . . 118.32(11) ?
V1 Mn1 O1 1_666 . 2_656 45.75(5) ?
V1 Mn1 O2 1_666 . . 115.33(8) ?
V1 Mn1 O2 1_666 . 1_655 105.88(5) ?
V1 Mn1 O2 1_666 . 2_666 42.37(10) ?
V1 Mn1 O3 1_666 . . 113.91(6) ?
V1 Mn1 O3 1_666 . 2_766 41.83(8) ?
O1 Mn1 O1 . . 2_656 92.45(13) ?
O1 Mn1 O2 . . . 100.57(12) ?
O1 Mn1 O2 . . 1_655 58.97(9) ?
O1 Mn1 O2 . . 2_666 160.65(15) ?
O1 Mn1 O3 . . . 101.75(13) ?
O1 Mn1 O3 . . 2_766 90.92(13) ?
O1 Mn1 O2 2_656 . . 86.49(13) ?
O1 Mn1 O2 2_656 . 1_655 126.37(13) ?
O1 Mn1 O2 2_656 . 2_666 73.59(11) ?
O1 Mn1 O3 2_656 . . 159.57(8) ?
O1 Mn1 O3 2_656 . 2_766 72.69(11) ?
O2 Mn1 O2 . . 1_655 138.75(10) ?
O2 Mn1 O2 . . 2_666 92.04(12) ?
O2 Mn1 O3 . . . 104.96(14) ?
O2 Mn1 O3 . . 2_766 156.68(12) ?
O2 Mn1 O2 1_655 . 2_666 118.73(8) ?
O2 Mn1 O3 1_655 . . 53.46(13) ?
O2 Mn1 O3 1_655 . 2_766 64.44(10) ?
O2 Mn1 O3 2_666 . . 88.91(11) ?
O2 Mn1 O3 2_666 . 2_766 72.37(13) ?
O3 Mn1 O3 . . 2_766 92.28(12) ?
Mn1 V1 V1 1_444 . 2_445 80.60(3) ?
Mn1 V1 V1 1_444 . 2_545 80.17(3) ?
Mn1 V1 V1 1_444 . 2_555 83.18(4) ?
Mn1 V1 O1 1_444 . 1_455 118.05(9) ?
Mn1 V1 O1 1_444 . 2_545 51.25(9) ?
Mn1 V1 O2 1_444 . . 120.11(11) ?
Mn1 V1 O2 1_444 . 2_555 50.25(8) ?
Mn1 V1 O3 1_444 . 1_445 115.10(8) ?
Mn1 V1 O3 1_444 . 2_655 47.65(9) ?
V1 V1 V1 2_445 . 2_545 112.78(3) ?
V1 V1 V1 2_445 . 2_555 121.11(4) ?
V1 V1 O1 2_445 . 1_455 44.12(7) ?
V1 V1 O1 2_445 . 2_545 35.77(9) ?
V1 V1 O2 2_445 . . 144.32(11) ?
V1 V1 O2 2_445 . 2_555 88.57(7) ?
V1 V1 O3 2_445 . 1_445 97.91(8) ?
V1 V1 O3 2_445 . 2_655 116.95(6) ?
V1 V1 V1 2_545 . 2_555 119.43(3) ?
V1 V1 O1 2_545 . 1_455 137.77(14) ?
V1 V1 O1 2_545 . 2_545 85.75(11) ?
V1 V1 O2 2_545 . . 99.95(12) ?
V1 V1 O2 2_545 . 2_555 122.56(10) ?
V1 V1 O3 2_545 . 1_445 40.44(9) ?
V1 V1 O3 2_545 . 2_655 39.34(12) ?
V1 V1 O1 2_555 . 1_455 101.19(13) ?
V1 V1 O1 2_555 . 2_545 124.59(12) ?
V1 V1 O2 2_555 . . 44.39(12) ?
V1 V1 O2 2_555 . 2_555 40.96(6) ?
V1 V1 O3 2_555 . 1_445 139.74(7) ?
V1 V1 O3 2_555 . 2_655 89.99(11) ?
O1 V1 O1 1_455 . 2_545 79.88(11) ?
O1 V1 O2 1_455 . . 101.49(12) ?
O1 V1 O2 1_455 . 2_555 95.16(17) ?
O1 V1 O3 1_455 . 1_445 100.47(17) ?
O1 V1 O3 1_455 . 2_655 161.06(9) ?
O1 V1 O2 2_545 . . 168.98(17) ?
O1 V1 O2 2_545 . 2_555 83.63(13) ?
O1 V1 O3 2_545 . 1_445 92.41(13) ?
O1 V1 O3 2_545 . 2_655 81.18(11) ?
O2 V1 O2 . . 2_555 85.35(14) ?
O2 V1 O3 . . 1_445 98.05(14) ?
O2 V1 O3 . . 2_655 97.20(12) ?
O2 V1 O3 2_555 . 1_445 162.96(13) ?
O2 V1 O3 2_555 . 2_655 83.24(15) ?
O3 V1 O3 1_445 . 2_655 79.77(15) ?
Mn1 O1 Mn1 . . 2_656 87.55(11) ?
Mn1 O1 V1 . . 1_655 119.04(15) ?
Mn1 O1 V1 . . 2_545 127.64(18) ?
Mn1 O1 O1 . . 2_645 149.0(2) ?
Mn1 O1 O1 . . 2_656 46.67(9) ?
Mn1 O1 O2 . . 1_545 138.02(15) ?
Mn1 O1 O2 . . . 39.29(8) ?
Mn1 O1 O2 . . 1_655 81.85(11) ?
Mn1 O1 O2 . . 2_655 92.56(15) ?
Mn1 O1 O2 . . 2_656 95.30(11) ?
Mn1 O1 O3 . . 1_445 88.62(14) ?
Mn1 O1 O3 . . 1_545 134.39(10) ?
Mn1 O1 O3 . . . 39.01(8) ?
Mn1 O1 O3 . . 2_655 93.36(16) ?
Mn1 O1 O3 . . 2_766 45.79(9) ?
Mn1 O1 V1 2_656 . 1_655 139.4(2) ?
Mn1 O1 V1 2_656 . 2_545 83.00(10) ?
Mn1 O1 O1 2_656 . 2_645 115.76(15) ?
Mn1 O1 O1 2_656 . 2_656 40.88(9) ?
Mn1 O1 O2 2_656 . 1_545 52.42(9) ?
Mn1 O1 O2 2_656 . . 86.13(12) ?
Mn1 O1 O2 2_656 . 1_655 130.81(13) ?
Mn1 O1 O2 2_656 . 2_655 173.62(14) ?
Mn1 O1 O2 2_656 . 2_656 43.00(8) ?
Mn1 O1 O3 2_656 . 1_445 51.27(10) ?
Mn1 O1 O3 2_656 . 1_545 97.94(16) ?
Mn1 O1 O3 2_656 . . 125.09(12) ?
Mn1 O1 O3 2_656 . 2_655 103.92(11) ?
Mn1 O1 O3 2_656 . 2_766 75.96(10) ?
V1 O1 V1 1_655 . 2_545 100.12(12) ?
V1 O1 O1 1_655 . 2_645 56.00(10) ?
V1 O1 O1 1_655 . 2_656 150.60(11) ?
V1 O1 O2 1_655 . 1_545 101.61(17) ?
V1 O1 O2 1_655 . . 134.1(2) ?
V1 O1 O2 1_655 . 1_655 40.25(8) ?
V1 O1 O2 1_655 . 2_655 45.23(12) ?
V1 O1 O2 1_655 . 2_656 100.78(17) ?
V1 O1 O3 1_655 . 1_445 146.89(12) ?
V1 O1 O3 1_655 . 1_545 41.51(12) ?
V1 O1 O3 1_655 . . 81.50(13) ?
V1 O1 O3 1_655 . 2_655 104.30(14) ?
V1 O1 O3 1_655 . 2_766 100.20(10) ?
V1 O1 O1 2_545 . 2_645 44.12(8) ?
V1 O1 O1 2_545 . 2_656 108.14(12) ?
V1 O1 O2 2_545 . 1_545 46.03(9) ?
V1 O1 O2 2_545 . . 88.61(12) ?
V1 O1 O2 2_545 . 1_655 139.30(14) ?
V1 O1 O2 2_545 . 2_655 91.91(11) ?
V1 O1 O2 2_545 . 2_656 110.88(15) ?
V1 O1 O3 2_545 . 1_445 46.78(8) ?
V1 O1 O3 2_545 . 1_545 97.95(14) ?
V1 O1 O3 2_545 . . 133.59(17) ?
V1 O1 O3 2_545 . 2_655 41.01(9) ?
V1 O1 O3 2_545 . 2_766 157.92(15) ?
O1 O1 O1 2_645 . 2_656 151.42(12) ?
O1 O1 O2 2_645 . 1_545 63.74(12) ?
O1 O1 O2 2_645 . . 118.14(15) ?
O1 O1 O2 2_645 . 1_655 95.67(13) ?
O1 O1 O2 2_645 . 2_655 61.97(12) ?
O1 O1 O2 2_645 . 2_656 115.61(19) ?
O1 O1 O3 2_645 . 1_445 90.89(10) ?
O1 O1 O3 2_645 . 1_545 65.60(13) ?
O1 O1 O3 2_645 . . 118.44(15) ?
O1 O1 O3 2_645 . 2_655 62.56(12) ?
O1 O1 O3 2_645 . 2_766 154.90(16) ?
O1 O1 O2 2_656 . 1_545 92.46(13) ?
O1 O1 O2 2_656 . . 56.21(11) ?
O1 O1 O2 2_656 . 1_655 112.52(9) ?
O1 O1 O2 2_656 . 2_655 138.84(17) ?
O1 O1 O2 2_656 . 2_656 61.83(11) ?
O1 O1 O3 2_656 . 1_445 61.89(9) ?
O1 O1 O3 2_656 . 1_545 123.97(15) ?
O1 O1 O3 2_656 . . 84.81(11) ?
O1 O1 O3 2_656 . 2_655 102.33(13) ?
O1 O1 O3 2_656 . 2_766 50.70(8) ?
O2 O1 O2 1_545 . . 115.80(12) ?
O2 O1 O2 1_545 . 1_655 131.84(19) ?
O2 O1 O2 1_545 . 2_655 125.71(12) ?
O2 O1 O2 1_545 . 2_656 65.41(12) ?
O2 O1 O3 1_545 . 1_445 58.04(12) ?
O2 O1 O3 1_545 . 1_545 71.42(13) ?
O2 O1 O3 1_545 . . 176.89(15) ?
O2 O1 O3 1_545 . 2_655 85.90(11) ?
O2 O1 O3 1_545 . 2_766 120.61(16) ?
O2 O1 O2 . . 1_655 112.29(15) ?
O2 O1 O2 . . 2_655 89.92(15) ?
O2 O1 O2 . . 2_656 118.05(13) ?
O2 O1 O3 . . 1_445 57.77(12) ?
O2 O1 O3 . . 1_545 172.64(12) ?
O2 O1 O3 . . . 61.38(11) ?
O2 O1 O3 . . 2_655 55.99(10) ?
O2 O1 O3 . . 2_766 83.44(12) ?
O2 O1 O2 1_655 . 2_655 55.44(10) ?
O2 O1 O2 1_655 . 2_656 90.24(12) ?
O2 O1 O3 1_655 . 1_445 170.0(2) ?
O2 O1 O3 1_655 . 1_545 60.44(12) ?
O2 O1 O3 1_655 . . 50.92(11) ?
O2 O1 O3 1_655 . 2_655 124.47(16) ?
O2 O1 O3 1_655 . 2_766 62.41(9) ?
O2 O1 O2 2_655 . 2_656 143.23(14) ?
O2 O1 O3 2_655 . 1_445 122.35(15) ?
O2 O1 O3 2_655 . 1_545 86.54(14) ?
O2 O1 O3 2_655 . . 56.51(10) ?
O2 O1 O3 2_655 . 2_655 69.70(11) ?
O2 O1 O3 2_655 . 2_766 108.58(11) ?
O2 O1 O3 2_656 . 1_445 93.75(14) ?
O2 O1 O3 2_656 . 1_545 62.70(12) ?
O2 O1 O3 2_656 . . 114.34(9) ?
O2 O1 O3 2_656 . 2_655 145.10(13) ?
O2 O1 O3 2_656 . 2_766 56.53(11) ?
O3 O1 O3 1_445 . 1_545 129.46(17) ?
O3 O1 O3 1_445 . . 119.14(17) ?
O3 O1 O3 1_445 . 2_655 52.71(11) ?
O3 O1 O3 1_445 . 2_766 112.59(13) ?
O3 O1 O3 1_545 . . 111.37(12) ?
O3 O1 O3 1_545 . 2_655 128.16(12) ?
O3 O1 O3 1_545 . 2_766 91.57(12) ?
O3 O1 O3 . . 2_655 93.21(15) ?
O3 O1 O3 . . 2_766 58.54(10) ?
O3 O1 O3 2_655 . 2_766 139.04(18) ?
Mn1 O2 Mn1 1_455 . . 138.75(12) ?
Mn1 O2 Mn1 1_455 . 2_666 61.27(8) ?
Mn1 O2 V1 1_455 . . 75.79(9) ?
Mn1 O2 V1 1_455 . 2_555 81.79(12) ?
Mn1 O2 O1 1_455 . 1_455 39.18(8) ?
Mn1 O2 O1 1_455 . . 145.32(14) ?
Mn1 O2 O1 1_455 . 1_565 95.92(13) ?
Mn1 O2 O1 1_455 . 2_655 121.30(16) ?
Mn1 O2 O1 1_455 . 2_656 93.17(10) ?
Mn1 O2 O2 1_455 . 2_555 73.51(10) ?
Mn1 O2 O2 1_455 . 2_666 98.29(10) ?
Mn1 O2 O3 1_455 . 1_445 96.01(10) ?
Mn1 O2 O3 1_455 . 1_455 39.37(8) ?
Mn1 O2 O3 1_455 . . 148.06(11) ?
Mn1 O2 O3 1_455 . 2_655 116.65(9) ?
Mn1 O2 O3 1_455 . 2_666 40.21(7) ?
Mn1 O2 Mn1 . . 2_666 87.96(8) ?
Mn1 O2 V1 . . . 123.4(2) ?
Mn1 O2 V1 . . 2_555 126.40(14) ?
Mn1 O2 O1 . . 1_455 137.2(2) ?
Mn1 O2 O1 . . . 40.14(8) ?
Mn1 O2 O1 . . 1_565 85.35(11) ?
Mn1 O2 O1 . . 2_655 92.74(12) ?
Mn1 O2 O1 . . 2_656 50.51(10) ?
Mn1 O2 O2 . . 2_555 147.59(16) ?
Mn1 O2 O2 . . 2_666 46.82(8) ?
Mn1 O2 O3 . . 1_445 84.24(15) ?
Mn1 O2 O3 . . 1_455 136.96(12) ?
Mn1 O2 O3 . . . 37.81(9) ?
Mn1 O2 O3 . . 2_655 95.72(15) ?
Mn1 O2 O3 . . 2_666 98.58(12) ?
Mn1 O2 V1 2_666 . . 136.29(16) ?
Mn1 O2 V1 2_666 . 2_555 87.37(15) ?
Mn1 O2 O1 2_666 . 1_455 98.07(12) ?
Mn1 O2 O1 2_666 . . 126.57(12) ?
Mn1 O2 O1 2_666 . 1_565 54.00(9) ?
Mn1 O2 O1 2_666 . 2_655 107.94(15) ?
Mn1 O2 O1 2_666 . 2_656 75.94(10) ?
Mn1 O2 O2 2_666 . 2_555 118.73(18) ?
Mn1 O2 O2 2_666 . 2_666 41.14(8) ?
Mn1 O2 O3 2_666 . 1_445 131.63(15) ?
Mn1 O2 O3 2_666 . 1_455 52.23(9) ?
Mn1 O2 O3 2_666 . . 88.03(8) ?
Mn1 O2 O3 2_666 . 2_655 175.53(19) ?
Mn1 O2 O3 2_666 . 2_666 42.93(8) ?
V1 O2 V1 . . 2_555 94.65(12) ?
V1 O2 O1 . . 1_455 38.26(8) ?
V1 O2 O1 . . . 84.74(14) ?
V1 O2 O1 . . 1_565 144.98(19) ?
V1 O2 O1 . . 2_655 100.68(12) ?
V1 O2 O1 . . 2_656 99.95(16) ?
V1 O2 O2 . . 2_555 49.34(10) ?
V1 O2 O2 . . 2_666 152.84(19) ?
V1 O2 O3 . . 1_445 41.74(10) ?
V1 O2 O3 . . 1_455 98.93(14) ?
V1 O2 O3 . . . 135.62(15) ?
V1 O2 O3 . . 2_655 42.75(8) ?
V1 O2 O3 . . 2_666 98.13(12) ?
V1 O2 O1 2_555 . 1_455 96.33(14) ?
V1 O2 O1 2_555 . . 128.83(14) ?
V1 O2 O1 2_555 . 1_565 50.34(10) ?
V1 O2 O1 2_555 . 2_655 39.61(10) ?
V1 O2 O1 2_555 . 2_656 162.91(14) ?
V1 O2 O2 2_555 . 2_555 45.31(10) ?
V1 O2 O2 2_555 . 2_666 110.92(14) ?
V1 O2 O3 2_555 . 1_445 134.08(10) ?
V1 O2 O3 2_555 . 1_455 48.01(11) ?
V1 O2 O3 2_555 . . 88.66(12) ?
V1 O2 O3 2_555 . 2_655 88.39(12) ?
V1 O2 O3 2_555 . 2_666 112.94(17) ?
O1 O2 O1 1_455 . . 112.29(15) ?
O1 O2 O1 1_455 . 1_565 131.84(18) ?
O1 O2 O1 1_455 . 2_655 124.56(13) ?
O1 O2 O1 1_455 . 2_656 89.76(13) ?
O1 O2 O2 1_455 . 2_555 61.57(11) ?
O1 O2 O2 1_455 . 2_666 125.81(13) ?
O1 O2 O3 1_455 . 1_445 60.21(12) ?
O1 O2 O3 1_455 . 1_455 72.42(13) ?
O1 O2 O3 1_455 . . 172.27(18) ?
O1 O2 O3 1_455 . 2_655 80.98(10) ?
O1 O2 O3 1_455 . 2_666 62.21(9) ?
O1 O2 O1 . . 1_565 115.80(12) ?
O1 O2 O1 . . 2_655 90.08(13) ?
O1 O2 O1 . . 2_656 61.95(12) ?
O1 O2 O2 . . 2_555 114.32(13) ?
O1 O2 O2 . . 2_666 86.07(11) ?
O1 O2 O3 . . 1_445 52.10(10) ?
O1 O2 O3 . . 1_455 175.16(14) ?
O1 O2 O3 . . . 60.03(10) ?
O1 O2 O3 . . 2_655 57.57(11) ?
O1 O2 O3 . . 2_666 117.79(15) ?
O1 O2 O1 1_565 . 2_655 54.29(11) ?
O1 O2 O1 1_565 . 2_656 114.59(10) ?
O1 O2 O2 1_565 . 2_555 95.64(16) ?
O1 O2 O2 1_565 . 2_666 61.16(10) ?
O1 O2 O3 1_565 . 1_445 167.87(16) ?
O1 O2 O3 1_565 . 1_455 59.45(12) ?
O1 O2 O3 1_565 . . 55.79(11) ?
O1 O2 O3 1_565 . 2_655 123.65(15) ?
O1 O2 O3 1_565 . 2_666 96.37(12) ?
O1 O2 O1 2_655 . 2_656 143.23(14) ?
O1 O2 O2 2_655 . 2_555 62.99(11) ?
O1 O2 O2 2_655 . 2_666 104.84(11) ?
O1 O2 O3 2_655 . 1_445 120.05(13) ?
O1 O2 O3 2_655 . 1_455 86.15(16) ?
O1 O2 O3 2_655 . . 57.10(10) ?
O1 O2 O3 2_655 . 2_655 69.41(11) ?
O1 O2 O3 2_655 . 2_666 147.63(18) ?
O1 O2 O2 2_656 . 2_555 148.29(14) ?
O1 O2 O2 2_656 . 2_666 53.43(10) ?
O1 O2 O3 2_656 . 1_445 62.50(11) ?
O1 O2 O3 2_656 . 1_455 120.09(14) ?
O1 O2 O3 2_656 . . 87.11(11) ?
O1 O2 O3 2_656 . 2_655 108.37(16) ?
O1 O2 O3 2_656 . 2_666 56.33(12) ?
O2 O2 O2 2_555 . 2_666 155.01(19) ?
O2 O2 O3 2_555 . 1_445 89.84(12) ?
O2 O2 O3 2_555 . 1_455 66.52(13) ?
O2 O2 O3 2_555 . . 119.47(14) ?
O2 O2 O3 2_555 . 2_655 56.97(12) ?
O2 O2 O3 2_555 . 2_666 113.43(14) ?
O2 O2 O3 2_666 . 1_445 114.75(15) ?
O2 O2 O3 2_666 . 1_455 91.96(12) ?
O2 O2 O3 2_666 . . 56.96(8) ?
O2 O2 O3 2_666 . 2_655 142.47(16) ?
O2 O2 O3 2_666 . 2_666 64.15(8) ?
O3 O2 O3 1_445 . 1_455 132.63(13) ?
O3 O2 O3 1_445 . . 112.13(15) ?
O3 O2 O3 1_445 . 2_655 51.57(11) ?
O3 O2 O3 1_445 . 2_666 91.32(13) ?
O3 O2 O3 1_455 . . 115.23(14) ?
O3 O2 O3 1_455 . 2_655 123.49(14) ?
O3 O2 O3 1_455 . 2_666 64.99(13) ?
O3 O2 O3 . . 2_655 93.31(11) ?
O3 O2 O3 . . 2_666 121.11(9) ?
O3 O2 O3 2_655 . 2_666 138.42(13) ?
Mn1 O3 Mn1 . . 2_766 87.72(14) ?
Mn1 O3 V1 . . 1_665 117.70(16) ?
Mn1 O3 V1 . . 2_655 124.30(18) ?
Mn1 O3 O1 . . . 39.23(9) ?
Mn1 O3 O1 . . 1_565 82.17(12) ?
Mn1 O3 O1 . . 1_665 141.4(2) ?
Mn1 O3 O1 . . 2_655 88.38(10) ?
Mn1 O3 O1 . . 2_766 96.38(12) ?
Mn1 O3 O2 . . . 37.23(9) ?
Mn1 O3 O2 . . 1_655 87.17(16) ?
Mn1 O3 O2 . . 1_665 133.85(16) ?
Mn1 O3 O2 . . 2_655 90.42(12) ?
Mn1 O3 O2 . . 2_666 48.17(8) ?
Mn1 O3 O3 . . 2_765 143.38(11) ?
Mn1 O3 O3 . . 2_766 45.22(9) ?
Mn1 O3 V1 2_766 . 1_665 137.24(13) ?
Mn1 O3 V1 2_766 . 2_655 90.51(14) ?
Mn1 O3 O1 2_766 . . 89.13(14) ?
Mn1 O3 O1 2_766 . 1_565 129.12(12) ?
Mn1 O3 O1 2_766 . 1_665 56.04(10) ?
Mn1 O3 O1 2_766 . 2_655 175.76(17) ?
Mn1 O3 O1 2_766 . 2_766 43.29(9) ?
Mn1 O3 O2 2_766 . . 123.36(15) ?
Mn1 O3 O2 2_766 . 1_655 55.40(10) ?
Mn1 O3 O2 2_766 . 1_665 97.17(10) ?
Mn1 O3 O2 2_766 . 2_655 111.90(17) ?
Mn1 O3 O2 2_766 . 2_666 75.36(10) ?
Mn1 O3 O3 2_766 . 2_765 124.95(14) ?
Mn1 O3 O3 2_766 . 2_766 42.50(8) ?
V1 O3 V1 1_665 . 2_655 100.23(16) ?
V1 O3 O1 1_665 . . 132.68(11) ?
V1 O3 O1 1_665 . 1_565 38.03(10) ?
V1 O3 O1 1_665 . 1_665 99.46(16) ?
V1 O3 O1 1_665 . 2_655 46.59(10) ?
V1 O3 O1 1_665 . 2_766 97.12(14) ?
V1 O3 O2 1_665 . . 82.37(12) ?
V1 O3 O2 1_665 . 1_655 148.95(17) ?
V1 O3 O2 1_665 . 1_665 40.21(9) ?
V1 O3 O2 1_665 . 2_655 102.25(13) ?
V1 O3 O2 1_665 . 2_666 95.90(15) ?
V1 O3 O3 1_665 . 2_765 50.90(13) ?
V1 O3 O3 1_665 . 2_766 146.71(16) ?
V1 O3 O1 2_655 . . 85.09(13) ?
V1 O3 O1 2_655 . 1_565 135.41(18) ?
V1 O3 O1 2_655 . 1_665 52.04(9) ?
V1 O3 O1 2_655 . 2_655 90.29(11) ?
V1 O3 O1 2_655 . 2_766 118.81(12) ?
V1 O3 O2 2_655 . . 126.38(10) ?
V1 O3 O2 2_655 . 1_655 48.75(11) ?
V1 O3 O2 2_655 . 1_665 101.60(14) ?
V1 O3 O2 2_655 . 2_655 40.05(7) ?
V1 O3 O2 2_655 . 2_666 163.6(2) ?
V1 O3 O3 2_655 . 2_765 49.33(12) ?
V1 O3 O3 2_655 . 2_766 112.79(18) ?
O1 O3 O1 . . 1_565 111.37(12) ?
O1 O3 O1 . . 1_665 119.14(17) ?
O1 O3 O1 . . 2_655 86.79(10) ?
O1 O3 O1 . . 2_766 121.46(15) ?
O1 O3 O2 . . . 58.59(10) ?
O1 O3 O2 . . 1_655 56.66(11) ?
O1 O3 O2 . . 1_665 170.72(15) ?
O1 O3 O2 . . 2_655 54.07(10) ?
O1 O3 O2 . . 2_666 86.32(12) ?
O1 O3 O3 . . 2_765 117.06(12) ?
O1 O3 O3 . . 2_766 57.69(10) ?
O1 O3 O1 1_565 . 1_665 129.46(17) ?
O1 O3 O1 1_565 . 2_655 51.84(10) ?
O1 O3 O1 1_565 . 2_766 88.43(12) ?
O1 O3 O2 1_565 . . 52.79(10) ?
O1 O3 O2 1_565 . 1_655 168.02(14) ?
O1 O3 O2 1_565 . 1_665 59.35(12) ?
O1 O3 O2 1_565 . 2_655 117.87(12) ?
O1 O3 O2 1_565 . 2_666 60.97(12) ?
O1 O3 O3 1_565 . 2_765 87.39(17) ?
O1 O3 O3 1_565 . 2_766 110.86(13) ?
O1 O3 O1 1_665 . 2_655 127.29(16) ?
O1 O3 O1 1_665 . 2_766 67.41(9) ?
O1 O3 O2 1_665 . . 177.71(18) ?
O1 O3 O2 1_665 . 1_655 62.51(13) ?
O1 O3 O2 1_665 . 1_665 70.13(13) ?
O1 O3 O2 1_665 . 2_655 91.55(12) ?
O1 O3 O2 1_665 . 2_666 122.07(10) ?
O1 O3 O3 1_665 . 2_765 69.00(12) ?
O1 O3 O3 1_665 . 2_766 97.57(14) ?
O1 O3 O1 2_655 . 2_766 139.04(18) ?
O1 O3 O2 2_655 . . 53.19(10) ?
O1 O3 O2 2_655 . 1_655 122.70(12) ?
O1 O3 O2 2_655 . 1_665 86.75(15) ?
O1 O3 O2 2_655 . 2_655 66.44(11) ?
O1 O3 O2 2_655 . 2_666 103.20(13) ?
O1 O3 O3 2_655 . 2_765 58.29(11) ?
O1 O3 O3 2_655 . 2_766 133.58(12) ?
O1 O3 O2 2_766 . . 113.83(12) ?
O1 O3 O2 2_766 . 1_655 98.20(13) ?
O1 O3 O2 2_766 . 1_665 60.97(11) ?
O1 O3 O2 2_766 . 2_655 153.54(17) ?
O1 O3 O2 2_766 . 2_666 55.37(8) ?
O1 O3 O3 2_766 . 2_765 118.39(13) ?
O1 O3 O3 2_766 . 2_766 63.78(10) ?
O2 O3 O2 . . 1_655 115.23(14) ?
O2 O3 O2 . . 1_665 112.13(15) ?
O2 O3 O2 . . 2_655 86.69(9) ?
O2 O3 O2 . . 2_666 58.89(8) ?
O2 O3 O3 . . 2_765 111.43(13) ?
O2 O3 O3 . . 2_766 81.50(11) ?
O2 O3 O2 1_655 . 1_665 132.63(13) ?
O2 O3 O2 1_655 . 2_655 56.51(11) ?
O2 O3 O2 1_655 . 2_666 115.01(17) ?
O2 O3 O3 1_655 . 2_765 98.07(15) ?
O2 O3 O3 1_655 . 2_766 64.10(13) ?
O2 O3 O2 1_665 . 2_655 128.43(15) ?
O2 O3 O2 1_665 . 2_666 88.68(12) ?
O2 O3 O3 1_665 . 2_765 64.54(13) ?
O2 O3 O3 1_665 . 2_766 123.85(11) ?
O2 O3 O2 2_655 . 2_666 138.42(13) ?
O2 O3 O3 2_655 . 2_765 63.89(12) ?
O2 O3 O3 2_655 . 2_766 105.66(16) ?
O2 O3 O3 2_666 . 2_765 146.7(2) ?
O2 O3 O3 2_666 . 2_766 50.91(11) ?
O3 O3 O3 2_765 . 2_766 161.75(19) ?





#=======================================================================

# 11. STRUCTURE-FACTOR LIST


loop_
_publcif_info_exptl_table_extra_item
sin_theta_over_lambda_max



_publcif_funding_html            
;
;
_exptl_crystal_recrystallization_method 'high pressure high temperature'
_exptl_crystal_preparation       'Magnetic properties'
